Slideshare uses cookies to improve functionality and performance, and to provide you with relevant advertising. If you continue browsing the site, you agree to the use of cookies on this website. See our User Agreement and Privacy Policy.

Slideshare uses cookies to improve functionality and performance, and to provide you with relevant advertising. If you continue browsing the site, you agree to the use of cookies on this website. See our Privacy Policy and User Agreement for details.

Like this document? Why not share!

- AI and Machine Learning Demystified... by Carol Smith 139001 views
- The AI Rush by Jean-Baptiste Dumont 47290 views
- 10 facts about jobs in the future by Pew Research Cent... 32519 views
- 2017 holiday survey: An annual anal... by Deloitte United S... 61237 views
- Harry Surden - Artificial Intellige... by Harry Surden 23431 views
- Inside Google's Numbers in 2017 by Rand Fishkin 541316 views

1,139 views

Published on

License: CC Attribution License

No Downloads

Total views

1,139

On SlideShare

0

From Embeds

0

Number of Embeds

4

Shares

0

Downloads

175

Comments

0

Likes

2

No embeds

No notes for slide

- 1. International Journal of Advances in Engineering & Technology, Nov. 2012.©IJAET ISSN: 2231-1963 NANOFLUID THERMAL CONDUCTIVITY-A REVIEW Ravi Sankar.B1, Nageswara Rao. D2,Srinivasa Rao.Ch.3 1 Lecturer, Mechanical Engg. Deptt., R.V.R&J.C. College of Engg., Guntur, A.P, India. 2 Vice-Chancellor, Centurion University, Odisa, India 3 Associate Professor, Mechanical Engineering Department, Andhra University College of Engineering, Visakhapatnam, A.P. India.ABSTRACTThe fluids dispersed with nanoparticles known as nanofluids are promising for heat transfer enhancement dueto their high thermal conductivity. In the present study, a literature review of nanofluid thermal conductivity isperformed. The possible mechanisms are presented for the high thermal conductivity of nanofluids. The effect ofsome parameters such as particle volume fraction, particle size, and temperature on thermal conductivity ispresented. Theoretical models are explained, model predictions are compared with experimental data, anddiscrepancies are indicated.KEYWORDS: Thermal conductivity, Volume Fraction, Particle size, Temperature I. INTRODUCTIONCooling is one of the most important challenges facing numerous industrial sectors. Despite theconsiderable amount of research and development focusing on industrial heat transfer requirements,major improvements in cooling capabilities have been lacking because conventional heat transferfluids have poor heat transfer properties. One of the usual methods used to overcome this problem isto increase the surface area available for heat exchange, which usually leads to impractical orunacceptable increases in the size of the heat management system. Thus there is a current need toimprove the heat transfer capabilities of conventional heat transfer fluids.Choi et al. [1] reported that the nanofluids (the fluids engineered by suspending metallicnanoparticles in conventional heat transfer fluids) were proved to have high thermal conductivitiescompared to those of currently used heat transfer fluids, and leading to enhancement of heat transfer.Choi et al. [2] produced nanofluids by suspending nanotubes in oil and experimentation had carriedout to measure effective thermal conductivity of nanofluids. They reported a 150 % thermalconductivity enhancement of poly (α-olefin) oil with the addition of multiwalled carbon nanotubes(MWCNT) at 1 % volume fraction. The results showed that the measured thermal conductivity wasanomalously greater than theoretical predictions and is nonlinear with nanotube concentration. Whencompared to other nanofluids, the nanofluids with nanotubes provide the highest thermal conductivityenhancement.Yang et al [3] addressed the effects of dispersant concentration, dispersing energy, and nanoparticleloading on thermal conductivity and steady shear viscosity of nanotube-in-oil dispersions. Thermalconductivity enhancement 200% was observed for poly (α-olefin) oil containing 0.35 % (v/v)MWCNT. It was found that fluids with large scale agglomerates have high thermal conductivities.Dispersion energy, applied by sonication, can decrease agglomerate size, but also breaks thenanotubes, decreasing both the thermal conductivity and viscosity of nanotube dispersions.In the present work first experimental studies on thermal conductivity of nanofluids affected byparameters like volume fraction, particle size, temperature etc are presented followed by theoretical 13 Vol. 5, Issue 1, pp. 13-28
- 2. International Journal of Advances in Engineering & Technology, Nov. 2012.©IJAET ISSN: 2231-1963models. Comparison of theoretical and experimental results is performed and possible mechanismsare explained for the discrepancy.II. EXISTING STUDIES ON NANOFLUID THERMAL CONDUCTIVITYStudies regarding the thermal conductivity of nanofluids showed that high enhancements of thermalconductivity than base fluids. It is possible to obtain larger thermal conductivity enhancements withlow particle volume fraction [4-8]. Such enhancement values exceed the predictions of theoreticalmodels developed for suspensions with larger particles. This is considered as an indication of thepresence of additional thermal transport enhancement mechanisms of nanofluids.2.1. Effect of particle Volume FractionThere are many studies in the literature about the effect of particle volume fraction of nanofluid,which is the volumetric concentration of the nanoparticles in the fluid, on the thermal conductivity.Eastman et al. [4] prepared Cu-ethylene glycol nanofluids and found that these fluids have muchhigher effective thermal conductivity than either pure ethylene glycol. The effective thermalconductivity of ethylene glycol was shown to be increased by up to 40% with an addition ofapproximately 0.3 vol. % Cu nanoparticles of mean diameter ≪10 nm. The addition of dispersantyielded a greater thermal conductivity than the same concentration of nanoparticles in the ethyleneglycol without the dispersant and no effect of either particle size or particle thermal conductivity wasobserved.Jana et al. [5] used conductive nanomaterials such as carbon nanotubes (CNTs), copper nanoparticles(Cu) and gold nanoparticles (Au), as well as their hybrids such as CNT-Cu or CNT-Au to enhance thethermal conductivity of fluids. They observed a 70 % thermal conductivity enhancement for 0.3 %(v/v) Cu nanoparticles in water. The results demonstrated that mono-type nanoparticle suspensionshave greatest enhancement in thermal conductivity, among which the enhancement with Cunanoparticle was the highest. The experimentally measured thermal conductivities of severalnanofluids were consistently greater than the theoretical predictions obtained from existing models.Liu et al [6] dispersed Cu nanoparticles in ethylene glycol, water, and synthetic engine oil usingchemical reduction method (one-step method). Experimental results illustrated that nanofluids withlow concentration of Cu have considerably higher thermal conductivity than those of base liquids. ForCu-water at 0.1 vol.%, thermal conductivity is increased by 23.8%. A strong dependence of thermalconductivity on the measured time was observed for Cu-water nanofluid.Murshed et al [7] prepared nanofluids by dispersing TiO2 nanoparticles (in rod-shapes and inspherical) shapes in deionized water. The experimental results demonstrated that the thermalconductivity increases with an increase of particle volume fraction. The particle size and shape alsohave effects on this enhancement of thermal conductivity.Zhu et al [8] studied thermal conductivitiesof Fe3O4 aqueous nanofluids. The results illustrated that Fe3O4 nanofluids have higher thermalconductivities than other oxide aqueous nanofluids at the same volume fraction. The experimentalvalues are higher than those predicted by the existing models. The abnormal thermal conductivitiesof Fe3O4 nanofluids are attributed to the observed nanoparticle clustering and alignment.Ceylan et al [9] prepared Ag-Cu alloy nanoparticles by the inert gas condensation (IGC) process. X-ray diffraction (XRD) patterns demonstrated that particles were phase separated as pure Cu and Agwith some Cu integrated in the Ag matrix. Thermal transport measurements have shown that there is alimit to the nanoparticle loading for the enhancement of the thermal conductivity. This maximumvalue was determined to be 0.006 vol. % of Ag-Cu nanoparticles, which led to the enhancement of thethermal conductivity of the pump oil by 33 percent.Zhang et al [10] measured the effective thermal conductivities and thermal diffusivities of Au/toluene,Al2O3/water, and carbon nanofiber (CNF)/water nanofluids and the influence of the volume fractionon thermal conductivity of the nanofluids was discussed. The measured results demonstrated that theeffective thermal conductivities of the nanofluids show no anomalous enhancements.Putnam et al [11] described an optical beam deflection technique for measurements of the thermaldiffusivity of fluid mixtures and suspensions of nanoparticles with a precision of better than 1%.Solutions of C60–C70fullerenes in toluene and suspensions of alkanethiolate-protected Aunanoparticles were measured to maximum volume fractions of 0.6% and 0.35 vol %, respectively. 14 Vol. 5, Issue 1, pp. 13-28
- 3. International Journal of Advances in Engineering & Technology, Nov. 2012.©IJAET ISSN: 2231-1963The largest increase in thermal conductivity they have observed was 1.3%±0.8% for 4 nm diameterAu particles suspended in ethanol.As seen in the Fig. 1, there exists significant discrepancy between experimental and theoretical data.This discrepancy can be explained by the fact that parameters such as PH of the nanofluid, dispersant,severity of clustering, and method of production of nanofluids usually differ in each experiment.Experimental results of Wen and Ding [59] are relatively higher than the results of other researchgroups and they are predicted best by the model of Koo and Kleinstreuer [57].However, since the size distribution of particles is not known in detail, it is difficult to reach aconclusion about the validity of the models. Dependency of the data of Lee et al. [21] on particlevolume fraction is somewhat low and none of the models have such a small slope in the figures.Hamilton and Crosser [54] model is relatively closer to the experimental data of Lee et al. [21] andDas et al. [15]. It was noted that clusters as large as 100 nm were observed in the study of Lee et al.[21]. Therefore, it may be suggested that those samples are closer to the validity range of theHamilton and Crosser model. However, Das et al. [15] also considered the effect of temperature intheir study and indicated that this agreement is just a coincidence. Figure 1. Comparison of the experimental results of the thermal conductivity ratio for Al 2O3 nanofluid with theoretical model as a function of particle volume fraction (Özerinç et al [23]).2.2. Effect of Particle SizeParticle size is another important parameter of thermal conductivity of nanofluids. It is possible toproduce nanoparticles of various sizes, generally ranging between 5 and 100 nm. Xie et al [12]prepared nanofluids containing Al2O3 nanoparticles with diameters in a range of 12 nm and 304 nm.Nanoparticle suspensions, containing a small amount of Al2O3, have significantly higher thermalconductivity than the base fluid. The enhanced thermal conductivity increases with an increase in thedifference between the PH value of aqueous suspension and the isoelectric point of Al2O3 particle.They concluded that there is an optimal particle size which yields the greatest thermal conductivityenhancement.Kim et al [13] measured thermal conductivity of water- and ethylene glycol-based nanofluidscontaining alumina, zinc-oxide, and titanium-dioxide nanoparticles using the transient hot-wire method. Measurements were conducted by varying the particle size and volume fraction. Fornanofluids containing 3 vol. % TiO2 in ethylene glycol, the thermal conductivity enhancement for the10 nm sample (16 %) was approximately double the enhancement for the 70 nm sample. The resultsillustrated that the thermal-conductivity enhancement ratio relative to the base fluid increases linearlywith decreasing the particle size but no existing empirical or theoretical correlation can explain thebehaviour.Li et al [14] used a steady state technique to evaluate the effective thermal conductivityofAl2O3∕distilled water nanofluids with nanoparticle diameters of 36 and 47 nm. Tests were conductedover a temperature range of 27–37 °C for volume fractions ranging from 0.5% to 6.0%. It was 15 Vol. 5, Issue 1, pp. 13-28
- 4. International Journal of Advances in Engineering & Technology, Nov. 2012.©IJAET ISSN: 2231-1963observed that up to 8 % greater thermal conductivity enhancement for aqueous nanofluids containing36 nm Al2O3 particles compared to nanofluids containing 47 nm Al2O3 particles. The thermalconductivity enhancement of the two nanofluids demonstrated a nonlinear relationship with respect totemperature, volume fraction, and nanoparticle size. Figure 2.Comparison of the experimental results of the thermal conductivity ratio for Al 2O3/water nanofluid with Hamilton and Crosser model [54] and Xue and Xu [46] as a function of the particle size at various values of the particle volume fraction (Özerinç et al [23]).The most significant finding was that the effect of variations in particle size had on the effectivethermal conductivity of the Al2O3∕distilled water nanofluids. The largest enhancement differenceobserved occurred at a temperature of approximately 32 °C and at a volume fraction of between 2%and 4%. From the experimental results it can be observed that an optimal size exists for differentnanoparticle and base fluid combinations.When Fig. 2 (Colours indicate different values of particle volume fraction; red 1%, brown 2%, blue3%, and black 4%)was observed, it was seen that Hamilton and model predicts increasing thermalconductivity with increasing particle size. The Hamilton and Crosser model [54] does not take theeffect of particle size on thermal conductivity into account, but it becomes slightly dependent onparticle size due to the fact that particle thermal conductivity increases with increasing particle size.However, the model still fails to predict experimental data for particle sizes larger than 40 nm sinceparticle size dependence diminishes with increasing particle size. This trend of increasing thermalconductivity with decreasing particle size is due to the fact that these models are either based onBrownian motion (Koo and Kleinstreuer [57] and Jang and Choi [31] models) or based on liquidlayering around nanoparticles (Yu and Choi [55], Xie et al. [29], Xue and Xu [46], and Sitprasert et al.[56] models). Fig.2 demonstrates thermal conductivity ratio for Al2O3/water nanofluid with Xue andXu model [46] as a function of the particle size at various values of the particle volume fraction.Colors indicate different values of particle volume fraction; red 1%, brown 2%, blue 3%, and black4%. Whereas Xue and Xu [46] model illustrates the trend of increasing thermal conductivity withdecreasing particle size is due to the fact that these models are either based on Brownian motion (Kooand Kleinstreuer [57] and Jang and Choi [31] models) or based on liquid layering aroundnanoparticles (Yu and Choi [55], Xie et al. [39], Xue and Xu [46], and Sitprasert et al. [56] models).Although the general trend for Al2O3/water nanofluids was as presented, there is also experimentaldata for Al2O3/water nanofluids, which shows increasing thermal conductivity with decreasingparticle size [19, 20, 61, 32, 35, and 58]. It should be noted that clustering may increase or decreasethe thermal conductivity enhancement. If a network of nanoparticles is formed as a result ofclustering, this may enable fast heat transport along nanoparticles. On the other hand, excessiveclustering may result in sedimentation, which decreases the effective particle volume fraction of thenanofluid. 16 Vol. 5, Issue 1, pp. 13-28
- 5. International Journal of Advances in Engineering & Technology, Nov. 2012.©IJAET ISSN: 2231-1963 Figure 3. Comparison of the experimental results of the thermal conductivity ratio for Al2O3/water nanofluid with Koo and Kleinstreuer model [57] and Jang and Choi model [31] as a function of temperature at various values of particle volume fraction. Colors indicate different values of particle volume fraction; red 1%, brown 2%, blue 3%, and black 4% (Özerinç et al [23]).2.3. Effect of TemperatureIn conventional suspensions of solid particles (with sizes on the order of millimeters or micrometers)in liquids, thermal conductivity of the mixture depends on temperature only due to the dependence ofthermal conductivity of base liquid and solid particles on temperature. Das et al [15] investigatedthe increase of thermal conductivity with temperature for nanofluids with water as base fluid andparticles of Al2O3 or CuO as suspension material. A temperature oscillation technique was used for themeasurement of thermal diffusivity and thermal conductivity. The results indicated an increase ofenhancement characteristics with temperature, within the limited temperature range consideredgradual curve appeared as linear.Yang et al [16] studied the temperature dependence of thermal conductivity enhancement innanofluids containing Bi2Te3 nanorods of 20nm in diameter and 170mm in length. The 3ω-wiremethod had been developed for measurement of the thermal conductivity of nanofluids. The thermalconductivity enhancement of nanofluids has been experimentally found to decrease with increasingtemperature, in contrast to the trend observed in nanofluids containing spherical nanoparticles. Theyobserved a decrease in the effective thermal conductivity as the temperature increased from 5 to 50ºC. The contrary trend was featured mainly to the particle aspect ratio.Honorine et al [17] reported effective thermal conductivity measurements of alumina/water andcopper oxide/water nanofluids. The effects of particle volume fraction, temperature and particle sizewere investigated. Readings at ambient temperature as well as over a relatively large temperaturerange were made for various particle volume fractions up to 9%. Results clearly illustrated that thepredicted overall effect of an increase in the effective thermal conductivity with an increase in particlevolume fraction and with a decrease in particle size. Furthermore, the relative increase in thermalconductivity was found to be more important at higher temperatures.The experimental results From Fig. 3 it should be noted that the presented data of Li and Peterson [18]was obtained by using the line fit provided by the authors since data points create ambiguity due tofluctuations. In the models, particle size is selected as 40 nm since most of the experimental data isclose to that value, as explained in the previous sections suggests that thermal conductivity ratioincreases with temperature. It is seen that the temperature dependence of the data of Li and Peterson[18] is much higher than the results of other two research groups. On the other hand, the results ofChon et al. [32] show somewhat weaker temperature dependence. This might be explained by the factthat the average size of nanoparticles in that study is larger when compared to others, since increasingparticle size decreases the effect of both Brownian motion and nanolayer formation. It should also benoted that dependence on particle volume fraction becomes more pronounced with increasingtemperature in all of the experimental studies [18].When it comes to theoretical models, predictions of Hamilton and Crosser model [54], Yu and Choimodel [55], Xue and Xu model [46], and Xie et al. [29] model does not depend on temperature exceptfor a very slight decrease in thermal conductivity ratio with temperature due to the increase in thethermal conductivity of water with temperature. Therefore, these models fail to predict the mentioned 17 Vol. 5, Issue 1, pp. 13-28
- 6. International Journal of Advances in Engineering & Technology, Nov. 2012.©IJAET ISSN: 2231-1963trends of experimental data. Since the predictions of these four models with respect to temperature donot provide any additional information; associated plots are not shown here.The model proposed by Koo and Kleinstreuer [57] considered the effect of Brownian motion on thethermal conductivity and the predictions of this model are presented in Fig. 3. The presented model ofKoo and Kleinstreuer predicts the trend in the experimental data correctly. The model proposed byJang and Choi [31] was presented in Fig. 3. Itwas noted that this model predicts nonlinear temperature dependence of thermal conductivity,whereas other two models predict linear behavior. Experimental results of Das et al. [15] and Li andPeterson [18] show nearly linear variation of thermal conductivity ratio with temperature, which iscontradictory with the model. On the other hand, result of Chon et al. [32] suggests nonlinearvariation and the associated trend is somewhat in agreement with the model of Jang and Choi.III. NANOFLUID THERMAL CONDUCTIVITY MODELSThe thermal conductivity enhancement of nanofluids was higher than those predicted fromconventional models for larger size particle dispersions as in Fig.4. Therefore, different researchers(Keblinski et.al [27] Li and Xuan [28]) Xie etal [29]) explored the mechanisms of heat transfer innanofluids, and proposed four possible reasons for the contribution of the system: 1. Brownian motion of the particle 2. Molecular-level layering of the liquid at the liquid/solid interface 3. The nature of the heat transport in nanoparticles 4. The effects of nanoparticles clustering Figure 4. Comparison of conventional models with the experimental dataKeblinski et al [27] investigated the effect of nanoparticle size on thermal conductivity of nanofluids.Thermal conductivity was found to be increased with the reduction in grain size of nanoparticleswithin the nanofluid. They concluded that the key factors for thermal properties of nanofluids are theballistic, rather than diffusive, nature of heat transport in the nanoparticles, combined with direct orfluid-mediated clustering effects that provide paths for rapid heat transport.Krischer [30] developed an empirical model to describe the irregular arrangement of suspendedparticles. The greater surface area associated with smaller particles promotes heat conduction. Thehigher specific surface area of nanoparticles improves a greater degree of aggregation than with asuspension of larger particles. Most nanofluid thermal conductivity models were developed based onone or more of these mechanisms.3.1. Brownian motionJang et al [31] found that the Brownian motion of nanoparticles at the molecular and nanoscale levelis a key mechanism governing the thermal behavior of nanofluids. They used a theoretical model thataccounts for the fundamental role of dynamic nanoparticles in nanofluids. The model not onlycaptures the concentration and temperature-dependent conductivity, but also predicts strongly size-dependent conductivity. The model is based on a linear combination of contributions from the liquid,the suspended particles, and the Brownian motion of the particles to give: 18 Vol. 5, Issue 1, pp. 13-28
- 7. International Journal of Advances in Engineering & Technology, Nov. 2012.©IJAET ISSN: 2231-1963 keff,m df 1 C1 Re2 Pr k1 d (1)where ε is a constant related to the Kapitza resistance, C1 is a proportionality constant, df is thediameter of a fluid molecule, and Re and Pr are the Reynolds the Prandtl numbers of the fluid,respectively. The Reynolds number, Re, is defined by, k BT Re 3 2l f (2)where kB is the Boltzmann constant, lf is the mean free path of a fluid molecule, and ρ and μ are thedensity and viscosity of the fluid, respectively. Their model reflects strong temperature dependencedue to Brownian motion and a simple inverse relationship with the particle diameter.Based on the Jang and Choi model, Chon et al. [32] employed the Buckingham-Pi theorem to developthe following empirical correlation, 0.3690 keff,m df 1 64.7 0.7460 0.7476 Pr 0.9955 Re1.2321 k1 d (3)where the Reynolds and Prandtl numbers are the same as in the Jang and Choi model [31]. Theequation was fit to their measurements of aqueous nanofluids containing three sizes of aluminaparticles. However, their correlation was of limited use, since it was based on measurements over alimited temperature range (20 – 70 ºC) and it was fit to thermal conductivity data for a singlenanoparticle material in a single base fluid. Chon et al [32] did not demonstrated any ability of theirmodel to predict the thermal conductivity of other nanofluids. Other models are available that arefitted to similarly limited nanofluid data and include no consideration for the more conventionalthermal conductivity models [33-35]. However, some researchers have used conventionalheterogeneous thermal conductivity models as a starting point and extended these to include a particlesize dependence based on Brownian motion.Xuan et al [36] adopted the concepts of both the Langevin equation of the Brownian motion and theconcept of the stochastic thermal process to describe the temperature fluctuation of the nanoparticlessuspended in base fluids. They developed an extension of the Maxwell equation to include the microconvective effect of the dynamic particles and the heat transfer between the particles and fluid to give: keff,m 2 2 1 18 HAT k1 2 1 2 d 6 k1 (4)where H is the overall heat transfer coefficient between the particle and the fluid, A is thecorresponding heat transfer area, and τ is the comprehensive relaxation time constant. The heattransfer area should be proportional to the square of the diameter, thus the effective thermalconductivity is proportional to the inverse of the particle diameter to the fourth power. Such strongparticle size dependence has yet to be demonstrated experimentally. Additionally, the equationreduces to the Maxwell equation with increasing particle size. As discussed previously, thermalconductivity enhancements greater than those predicted by the Maxwell equation have been reportedfor nanofluids containing relatively large nanoparticles (d > 30 nm) [37]. It is therefore obvious thatmodels that reduce to the Maxwell equation at large nanoparticle sizes will not be able to representpublished data.Numerous thermal conductivity models have been developed for heterogeneous systems andspecifically for nanofluids. Theoretical models such as those by Maxwell [37] and Bruggeman [38]were derived by assuming a homogeneous or random arrangement of particles. However, theseassumptions are not valid for dispersions containing aggregates. Empirical models [20, 22] have beensuccessfully employed to account for the spatial arrangement of particles. More recently, particle sizehas been incorporated into many models in an attempt to describe the thermal conductivity ofnanofluids. Several mechanisms have been described that may affect the thermal conductivity ofnanofluids, including Brownian motion of the particles, ordered liquid molecules at the solid / liquid 19 Vol. 5, Issue 1, pp. 13-28
- 8. International Journal of Advances in Engineering & Technology, Nov. 2012.©IJAET ISSN: 2231-1963interface, nanoparticle clustering, and interfacial thermal resistance. However, there is no consent asto which mechanism has the dominant effect on the thermal conductivity.3.2. Interfacial layering of liquid moleculesNan, et al [39, 40] addressed the effect of interfacial resistance (Kapitza resistance) on thermalconductivity of particulate composites due to weak interfacial contact. They set up a theoretical modelto predict thermal conductivity of composites by including interfacial resistance. According to thismodel, the effective thermal conductivity should decrease with decrease of the nanoparticle sizewhich is contrary to most of the experiment results for nanofluids. Yu et al [41] reported thatmolecules of normal liquids close to a solid surface can organize into layered solid like structure. Thiskind of structure at interface is a governing factor in heat conduction from solid surface to liquid.Choi et al [42] pointed out that this mechanism contributed to anomalous thermal conductivityenhancement in nanotube dispersions. However, Keblinski et al [27] indicated that the thickness ofthe interfacial solid-like layer is too small to dramatically increase of the thermal conductivity ofnanofluids because a typical interfacial width is only on the order of a atomic distance (1nm). So thismechanism only can be applied to very small nanoparticles (<10nm).Xue [45, 46] developed a novel model which was based on Maxwell theory and average polarizationtheory for effective thermal conductivity of nanofluids by including interface effect between solidparticle and base liquid. In this work solid nanoparticle and interfacial shell (nanolayer of liquidmolecules) considered as a “complex nanoparticle” and set up the model based on this concept. Thetheoretical results obtained from this model were in good agreement with the experimental data foralumina nanoparticle dispersions (Xue, Wu et al. [46]) and showed nonlinear volume fractiondependence for thermal conductivity enhancement in nanotube dispersions. Ren, Xie et al. [47] andXie, Fujii et al.[48] investigated the effect of interfacial layer on the effective thermal conductivity ofnanofluids. A model has been derived from general solution of heat conduction equation and theequivalent hard sphere fluid model representing microstructure of particle suspensions. Theirsimulation work showed that the thermal conductivity of nanofluids increased with decrease of theparticle size and increase of nanolayer thickness. The calculating values were in agreement with someexperimental data (Lee, Choi et al. [42]; Eastman, Choi et al. [43]). Recently, a new thermalconductivity model for nanofluids was developed by Yu et al [49]. This model was based on theassumption that monosized spherical nanoparticle are uniformly dispersed in the liquid and arelocated at the vertexes of a simple cubic lattice, with each particle surrounded by an organized liquidlayer. A nonlinear dependence of thermal conductivity on particle concentration was showed by thismodel and the relationship changed from convex upward to concave upward.In order to find the connection between nanolayer at interface and the thermal conductivity ofnanofluids, Yu et al. [41] modified the Maxwell equation for spherical particles and Hamilton-Crosserequation for non-spherical particles to predict the thermal conductivity of nanofluid by including theeffect of this ordered nanolayer. The result was substituted into the Maxwell model and the followingexpression was obtained. k pe 2k f 2 k pe k f 1 3 knf kf k pe 2k f k pe k f 1 3 kf (5) where kpeis the thermal conductivity of the equivalent nanoparticle; 2 1 1 3 1 2 k pe k 1 1 3 1 2 p (6)Where kl kp (7)and k is thermal conductivity of the nanolayer. β is defined as: l 20 Vol. 5, Issue 1, pp. 13-28
- 9. International Journal of Advances in Engineering & Technology, Nov. 2012.©IJAET ISSN: 2231-1963 t rp (8)where t is nanolayer thickness and rpthe nanoparticle radius.Yu and Choi later applied the same idea to the Hamilton and Crosser [54] model and proposed amodel for nonspherical particles [65]. Another model that considers non-spherical particles wasdeveloped by Xue [66].Xie et al. [29] also studied the effect of the interfacial nanolayer on the enhancement of thermalconductivity with nanofluids. A nanolayer was modeled as a spherical shell with thickness t aroundthe nanoparticle similar to Yu et al [41]. However, the thermal conductivity was assumed to changelinearly across the radial direction, so that it is equal to thermal conductivity of base liquid at thenanolayer–liquid interface and equal to thermal conductivity of the nanoparticle at the nanolayer–nanoparticle interface. The associated expression for the determination of the thermal conductivity ofnanofluid was given as: knf k f 32T 2 3T kf 1 T (9)Where pl lf 1 3 fl 1 2 pl fl 3 (10)and kl k flf kl 2k f k p kl pl k p 2kl k f kl fl k f 2klwhere T is the total volume fraction of nanoparticles and nanolayers. kl is the thermal conductivity ofthe nanolayer, Tcan be determined usingT 1 3Where tr pkl was defined as: kf M 2kl M ln 1 M MWhereM p 1 1 p kp k fWhen the thermal conductivity of the nanolayer is taken as a constant, this model gives the sameresults as Yu and Choi [41] model. It was shown that for a chosen nanolayer thickness, the model is inagreement only with some of the experimental data. As a result, it was concluded that liquid layeringaround nanoparticles is not the only mechanism that affects the thermal conductivity of nanofluids. 21 Vol. 5, Issue 1, pp. 13-28
- 10. International Journal of Advances in Engineering & Technology, Nov. 2012.©IJAET ISSN: 2231-1963Xue and Xu [46] presented another theoretical study for the effective thermal conductivity ofnanofluids. In their derivation, nanoparticles were assumed to have a liquid layer around them with aspecific thermal conductivity. First, an expression for the effective thermal conductivity of the“complex particle,” which was defined as the combination of the nanoparticle and nanolayer, wasdetermined. Then, by using Bruggeman’s effective media theory [38], the effective thermalconductivity of the nanofluid was determined. The resulting implicit expression for thermalconductivity of nanofluids is knf k f knf kl 2kl k p k p kl 2kl knf 1 0 2knf k f 2knf kl 2kl k p 2 k p kl kl knf (11)where subscript l refers to nanolayer. α is defined as 3 r p r t p (12) where t is the thickness of the nanolayer.Li et al. [67] considered the effect of Brownian motion, liquid layering around nanoparticles, andclustering together. The effect of temperature on average cluster size, Brownian motion, andnanoparticle thermal conductivity was taken into account. Nanoparticle thermal conductivity iscalculated by using the following expression: 3r * 4 kp k 3r* 4 1 b (13)Here, k is thermal conductivity of the bulk material and r rp where λ is the mean-free path of * bphonons. Mean-free path of phonons can be calculated according to the following expression: 10aTm T (14)Here, a is crystal lattice constant of the solid, γ Gruneisen constant, T temperature, and Tmthe meltingpoint (in K). It is assumed that thermal conductivity of the nanolayer is equal to the thermalconductivity of nanoparticles. As a result, particle volume fraction is modified according to theexpression: eff 1 t rp 3 (15)rpis particle radius in this equation. The expressions presented above are substituted into the Xuan etal. [28] model (Eq. 16) to obtain:knf k p 2k f 2 k f k p p c p , p kBT kf k p 2k f k f k p 2k f 3 rcl f (16)Another study regarding the effect of nanolayers was made by Sitprasert et al. [56]. They modified themodel proposed by Leong et al. [68] by taking the effect of temperature on the thermal conductivityand thickness of nanolayer into account. Leong et al.’s static model is as follows: k p kl kl 213 3 1 k p 2kl 13 3 kl k f k f knf 13 k p 2kl k p kl 13 3 1 (17)Here, subscript l refers to nanolayer. β and β1are defined as: t 1 rp t1 1 2rp 22 Vol. 5, Issue 1, pp. 13-28
- 11. International Journal of Advances in Engineering & Technology, Nov. 2012.©IJAET ISSN: 2231-1963t is the thickness of the nanolayer and rpis the radius of the nanoparticles. This model was modifiedby providing the following relation for the determination of nanolayer thickness: t 0.01T 273 rp 0.35 (18)where T is temperature in K and rp the particle radius in nanometers. After the determination ofnanolayer thickness, thermal conductivity of the nanolayer should be found according to theexpression: t kl C kf rp (19)where C is 30 and 110 for Al O and CuO nanoparticles, respectively. It should be noted that the 2 3above expressions provided for the determination of the thickness and thermal conductivity of thenanolayer were determined by using experimental data (which is known to have great discrepanciesand uncertainties) and no explanation was made regarding the physics of the problem.When the theoretical models based on nanolayer formation around nanoparticles are considered, it isseen that the main challenge is finding the thermal conductivity and thickness of the nanolayer.3.3. Nature of heat transfer in nanoparticlesKeblinski et al [27] estimated the mean free path of a phonon in Al 2O3 crystal is ~35nm. Phonons candiffuse in the 10nm particles but have to move ballistically. In order to make the ballistic phononsinitiated in one nanoparticle to persist in the liquid and reach another nanoparticle, high packingfractions, soot-like particle assemblies, and Brownian motion of the particles will be necessary tokeep the separation among nanoparticles to be small enough. However, Xie et al. [12] found in theirresearch about alumina nanofluids that when the particle size close to the mean free paths of phonons,the thermal conductivity of nanofluid may decrease with particle size because the intrinsic thermalconductivity of nanoparticle was reduced by the scattering of phonon at particle boundary. However,this result was not in agreement with most of the experimental results from other groups. Choi et al[42] indicated that sudden transition from ballistic heat conduction in nanotubes to diffusion heatconduction in liquid would severely limit the contribution of ballistic heat conduction to overallthermal conductivity of nanotube dispersions. They suggested that both ballistic heat conduction andlayering of liquid molecules at interface contributed to the high thermal conductivity of nanotubedispersions. The nature of heat transfer in nanoparticles or the fast ballistic heat conduction cannot bethe mechanism works alone to explain thermal conductivity enhancement of nanofluids due to thebarrier caused by slow heat diffusion in liquid. Other mechanisms need to be combined with it to fullyunderstand the enhancement of the thermal conductivity in nanofluids.3.4. Nanoparticle clustersXuan et al. [38] studied the thermal conductivity of nanofluids by considering Brownian motion andclustering of nanoparticles. An equation was proposed to predict the thermal conductivity ofnanofluids: knf k p 2k f 2 k f k p p c p , p kBT kf k p 2k f k f k p 2k f 3 rcl f (18)Here, rcl is the apparent radius of the nanoparticle clusters, which should be determined by experiment.T is temperature in K. μf is the dynamic viscosity of the base fluid and it can be calculated from thestudy of Li and Xuan [36]. The first term on the right-hand side of Eq. (18) is the Maxwell model [37]for thermal conductivity of suspensions of solid particles in fluids. The second term on the right-handside of Eq. (18) adds the effect of the random motion of the nanoparticles into account. For thecontribution of this term, the following values were presented for Cu (50 nm)/water nanofluid: For φ= 0.03%, contribution of the second term is 11% when clustering occurs and 17% when clusteringdoes not occur. For φ = 0.04%, contribution of the second term is 14% when clustering occurs and24% when clustering does not occur. It was indicated that Brownian motion of nanoparticles becomes 23 Vol. 5, Issue 1, pp. 13-28
- 12. International Journal of Advances in Engineering & Technology, Nov. 2012.©IJAET ISSN: 2231-1963more effective with increasing temperature. On the other hand, as nanoparticles (or clusters) becomelarger, their random motion becomes slower and this decreases the enhancement in thermalconductivity. It should be noted that the second term on the right-hand side of the equation is notnondimensional, which is an indication of a mistake in the analysis.Chen et al. [63] measured the viscosity of TiO2/water and TiO2/ethylene glycol nanofluids andproposed a way of calculating the thermal conductivity of nanofluids by using the data. Two types ofnanoparticles were used; spherical particles (25 nm) and cylindrical particles (10 nm in diameter and100 nm in length). The model was found to be a function of cluster radius, and cluster radius values ofthe sample nanofluids were determined by matching the predictions of the modified model withexperimental data. Then, the determined cluster radius values were used in the thermal conductivitymodel proposed, which is a modification of Hamilton and Crosser [54] model . knf kcl n 1 k f n 1 cl k f kcl kf kcl n 1 k f cl k f kcl (19)where kcl and φclare the thermal conductivity and volume fraction of the clusters, respectively. n wastaken as 3 for the spheres and 5 for the cylinders in this work.cl rcl rp 3-Dwhere rcl and rp are the radii of the clusters and nanoparticles, respectively. D is the fractal index,which was taken as 1.8 in the viscosity model and the same value might be used here. rcl / rp values areequal to 2.75 and 3.34, for TiO2/water (spherical) and TiO2/ethylene glycol (spherical) nanofluids,respectively. For the estimation of kcl, the following expression was proposed for spherical particles[38]: kp 3in 1 3 1 in 1 kf kcl 1 2 1 k f 4 2 kp kp 3in 1 k 3 1 in 1 8 k f f (20)where in is the solid volume fraction of clusters and it is defined as D 3 in rcl r p For the estimation of kcl, the following expression was proposed for nanotubes [64]. kcl 3 in 2 x 1 Lx z 1 Lz kf 3 in 2 x Lx z Lz (21)Where x kx k f k f Lx kt k f (22)Where z kz k f k f Lz kt k f (23)kx and kz are the thermal conductivity of nanotubes along transverse and longitudinal directions,respectively. kt is the isotropic thermal conductivity of the nanotube kx, kz and kt can be taken to beequal to kp as an approximation. Lx and Lzare defined as: p2 p2Lx cosh 1 p 2 p 1 2 p 2 1 2 2 3 (24)WhereLz 1 2Lx 24 Vol. 5, Issue 1, pp. 13-28
- 13. International Journal of Advances in Engineering & Technology, Nov. 2012.©IJAET ISSN: 2231-1963rcl / rp values are equal to 5.40 and 12.98 for TiO2/ethylene glycol (nanotube) and TiO2/water(nanotube) nanofluids, respectively. p is the aspect ratio of the nanotubes defined as length ofnanotube divided by diameter of nanotube. The modified Hamilton and Crosser [44] model (Eqs. 2, 3)was compared with experimental data for both spherical particles and nanotubes, and a goodagreement was observed.IV. CONCLUSIONThe available literature on nanofluid was thoroughly reviewed in this article. Some of the mostrelevant experimental results were reported for thermal conductivity several nanofluids. Thermalconductivity was found to be increased with the increase in particle volume fraction of nanoparticles.However, Effect of particle size on the thermal conductivity of nanofluids has not been completelyunderstood yet. It is expected that Brownian motion of nanoparticles results in higher thermalconductivity enhancement with smaller particle size. However, some of the experiments show that thethermal conductivity decreases with decreasing particle size. This contradiction might be due to theuncontrolled clustering of nanoparticles resulting in larger particles. Particle size distribution ofnanoparticles is another important factor and it is suggested that average particle size is not sufficientto characterize a nanofluid due to the nonlinear relations involved between particle size and thermaltransport. Temperature dependence is an important parameter in the thermal conductivity ofnanofluids. Limited study has been done about this aspect of the thermal conductivity of nanofluidsup to now. Investigation of the thermal performance of nanofluids at high temperatures may widen thepossible application areas of nanofluids. V. SCOPE FOR FUTURE WORKThe experimental results show that there exists significant discrepancy in the experimental data fornanofluid properties. An important reason of discrepancy in experimental data is the clustering ofnanoparticles. Although there are no universally accepted quantitative values, it is known that thelevel of clustering affects the properties of nanofluids. Since level of clustering is related to the pHvalue and the additives used, two nanofluid samples with all of the parameters being the same canlead to completely different experimental results if their surfactant parameters and pH values are notthe same. Therefore, the researchers providing experimental results should give detailed informationabout the additives utilized and pH values of the samples.REFERENCES[1]. S. Choi, , “Enhancing thermal conductivity of fluids with nanoparticles”, In Development and Applicationsof Non-Newtonian Flows, Ed. D A Siginer, H P Wang, New York: ASME. 1995 pp 99-105.[2]. Choi, S.U.S., Z.G. Zhang, W. Yu, F.E. Lockwood, and E.A. Grulke” Anomalous thermal conductivityenhancement in nanotube suspensions,” Applied Physics Letters, 2001. 79(14): p. 2252-2254.[3]. Yang, Y., E.A. Grulke, Z.G. Zhang, and G.F. Wu, “Thermal and rheological properties of carbon nanotube-in-oil dispersions,” Journal of Applied Physics, 2006. 99(11).[4]. Eastman, J.A., S.U.S. Choi, S. Li, W. Yu, and L.J. Thompson “Anomalously increased effective thermalconductivities of ethylene glycol-based nanofluids containing copper nanoparticles,” Applied Physics Letters,2001. 78(6): p. 718- 720.[5]. Jana, S., A. Salehi-Khojin, and W.H. Zhong “Enhancement of fluid thermal conductivity by the addition ofsingle and hybrid nano-additives,” Thermochimica Acta, 2007. 462(1-2): p. 45-55.[6]. Liu, M.S., M.C.C. Lin, C.Y. Tsai, and C.C. Wang “Enhancement of thermal conductivity with Cu fornanofluids using chemical reduction method,” International Journal of Heat and Mass Transfer, 2006. 49(17-18): p. 3028-3033.[7]. Murshed, S.M.S., K.C. Leong, and C. Yang”Enhanced thermal conductivity of TiO2 - water basednanofluids,” International Journal of Thermal Sciences, 2005. 44(4): p. 367-373.[8]. Zhu, H.T., C.Y. Zhang, S.Q. Liu, Y.M. Tang, and Y.S. Yin” Effects of nanoparticle clustering andalignment on thermal conductivities of Fe3O4 aqueous nanofluid ,” Applied Physics Letters, 2006. 89(2).[9]. Ceylan, A., K. Jastrzembski, and S.I. Shah “Enhanced solubility Ag-Cu nanoparticles and their thermaltransport properties,” Metallurgical and Materials Transactions a-Physical Metallurgy and Materials Science,2006. 37A(7): p. 2033-2038. 25 Vol. 5, Issue 1, pp. 13-28
- 14. International Journal of Advances in Engineering & Technology, Nov. 2012.©IJAET ISSN: 2231-1963[10]. Zhang, X., H. Gu, and M. Fujii ‘Effective thermal conductivity and thermal diffusivity of nanofluidscontaining spherical and cylindrical nanoparticles,” Journal of Applied Physics, 2006. 100(4): p. 044325.[11]. Putnam, S.A., D.G. Cahill, P.V. Braun, Z.B. Ge, and R.G. Shimmin “Thermal conductivity of nanoparticlesuspensions,” Journal of Applied Physics, 2006. 99(8)[12]. Xie, H.Q., J.C. Wang, T.G. Xi, Y. Liu, F. Ai, and Q.R. Wu ,”Thermal conductivity enhancement ofsuspensions containing nanosized alumina particles,” Journal of Applied Physics, 2002. 91(7): p. 4568-4572.[13]. Kim, S.H., S.R. Choi, and D. Kim “Thermal conductivity of metal-oxide nanofluids: Particle sizedependence and effect of laser irradiation,” Journal of Heat Transfer-Transactions of the ASME, 2007. 129(3):p. 298-307.[14]. Li, C.H. and G.P. Peterson ” The effect of particle size on the effective thermal conductivity of Al2O3-water nanofluid,” Journal of Applied Physics, 2007. 101(4): p. 044312.[15]. Das, S.K., N. Putra, P. Thiesen, and W. Roetzel “Temperature dependence of thermal conductivityenhancement for nanofluids,” Journal of Heat Transfer- Transactions of the ASME, 2003. 125(4): p. 567-574.[16]. Yang, B. and Z.H. Han “Temperature-dependent thermal conductivity of nanorodbased nanofluids,”Applied Physics Letters, 2006. 89(8).[17]. Honorine Angue Mintsa, Gilles Roy, Cong Tam Nguyen, Dominique Doucet, “ New temperaturedependent thermal conductivity data for water-based nanofluids” International Journal of Thermal Sciences,Volume 48, Issue 2, February 2009, Pages 363–371.[18]. Li, C.H. and G.P. Peterson” Experimental investigation of temperature and volume fraction variations onthe effective thermal conductivity of nanoparticle suspensions (nanofluids),” Journal of Applied Physics, 2006.99(8).[19]. Eastman, J.A., U.S. Choi, S. Li, L.J. Thompson, and S. Lee” Enhanced thermal conductivity through thedevelopment of nanofluids,” Materials Research Society Symposium Proceedings, 1997. 457(Nanophase andNanocomposite Materials II): p. 3-11.[20]. Wang, X.W., X.F. Xu, and S.U.S. Choi “Thermal conductivity of nanoparticle-fluid mixture,” Journal ofThermophysics and Heat Transfer, 1999. 13(4): p. 474- 480.[21]. Lee, S., S.U.S. Choi, S. Li, and J.A. Eastman” Measuring thermal conductivity of fluids containing oxidenanoparticles,” Journal of Heat Transfer-Transactions of the ASME, 1999. 121(2): p. 280-289.[22]. Hwang, Y.J., Y.C. Ahn, H.S. Shin, C.G. Lee, G.T. Kim, H.S. Park, and J.K. Lee, “Investigation oncharacteristics of thermal conductivity enhancement of nanofluids,” Current Applied Physics, 2006. 6(6): p.1068-1071.[23]. Özerinç, S., Kakaç, S., and Yazıcıoğlu, A. G., , “Enhanced Thermal Conductivity of Nanofluids: A State-of-the-Art Review,” Microfluid. Nanofluid., 2010 8(2), pp. 145-170.[24]. Wright, B., D. Thomas, H. Hong, L. Groven, J. Puszynski, E. Duke, X. Ye, and S. Jin “Magnetic fieldenhanced thermal conductivity in heat transfer nanofluids containing Ni coated single wall carbon nanotubes,”Applied Physics Letters, 2007.[25]. Hong, H.P., B. Wright, J. Wensel, S.H. Jin, X.R. Ye, and W. Roy “Enhanced thermal conductivity by themagnetic field in heat transfer nanofluids containing carbon nanotube,” Synthetic Metals, 2007. 157(10-12): p.437-440.[26]. Wensel, J., B. Wright, D. Thomas, W. Douglas, B. Mannhalter, W. Cross, H.P. Hong, J. Kellar, P. Smith,and W. Roy “Enhanced thermal conductivity by aggregation in heat transfer nanofluids containing metal oxidenanoparticles and carbon nanotubes,” Applied Physics Letters, 2008.[27]. Keblinski, P., S.R. Phillpot, S.U.S. Choi, and J.A. Eastman “Mechanisms of heat flow in suspensions ofnano-sized particles (nanofluids),” International Journal of Heat and Mass Transfer, 2002. 45(4): p. 855-863.[28]. Xuan, Y., Li, Q., Hu, W., Aggregation structure and Thermal conductivity of Nanofluids, AIchE Journal,vol. 49, no. 4, 2003, pp. 1038-1043.[29]. Xie, H., Fujii, M., and Zhang, X., Effect of interfacial Nanolayer on the effective thermal conductivity ofNanoparticle fluid Mixture, International Journal of Heat and Mass transfer, vol. 48, 2005, pp.2926-2932.[30]. Krischer, O., Die wissenschaftlichen Grundlagen der Trocknungstechnik (The Scientific Fundamentals ofDrying Technology). 2nd ed. 1963, Berlin: Springer- Verlag[31]. Jang, S.P. and S.U.S. Choi “Role of Brownian motion in the enhanced thermal conductivity of nanofluids,”Applied Physics Letters, 2004. 84(21): p. 4316-4318.[32]. Chon, C.H., K.D. Kihm, S.P. Lee, and S.U.S. Choi “Empirical correlation finding the role of temperatureand particle size for nanofluid (Al2O3) thermal conductivity enhancement ,”Applied Physics Letters, 2005.87(15).[33]. Turian, R.M., D.J. Sung, and F.L. Hsu” Thermal conductivity of granular coals, coal-water mixtures andmulti-solid/liquid suspensions,” Fuel, 1991. 70(10): p. 1157-1172.[34]. Patel, H.E., T. Sundararajan, T. Pradeep, A. Dasgupta, N. Dasgupta, and S.K. Das” A micro-convectionmodel for thermal conductivity of nanofluids,” Pramana- Journal of Physics, 2005. 65(5): p. 863-869. 26 Vol. 5, Issue 1, pp. 13-28
- 15. International Journal of Advances in Engineering & Technology, Nov. 2012.©IJAET ISSN: 2231-1963[35]. Patel, H.E., T. Sundararajan, and S.K. Das “A cell model approach for thermal conductivity ofnanofluids,” Journal of Nanoparticle Research, 2008. 10(1): p. 87- 97.[36]. Xuan, Y.M., Q. Li, X. Zhang, and M. Fujii “Stochastic thermal transport of nanoparticle suspensions,”Journal of Applied Physics, 2006. 100(4).[37]. Maxwell, J.C., A Treatise on Electricity and Magnetism. 3rd ed. Vol. II. 1892, London: oxford UniversityPress.[38]. Bruggeman, D.A.G., “Calculation of various physics constants in heterogenous substances I Dielectricityconstants and conductivity of mixed bodies from isotropic substances”, Annalen Der Physik, 1935. 24(7): p.636-664.[39]. Nan, C.W., Liu, G., Lin, Y., Li., M., “Interface effective thermal conductivity of carbon nanotubecomposites”, Applied Physics Letters, vol. 85, 2004, pp.3549-3551.[40].Nan, C.W., Birringer, R.,” Effective Thermal conductivity of particulate composites with interfacialthermal resistance”, Journal of Applied Physics, vol. 81, 1997, pp.6692-6699.[41]. Yu, C.J., Richter, A.G., Datta, A., Durbin, M.K., Dutta, P., “Molecular layering in a liquid on a solidsubstrate: An x-Ray reflectivity study”, Physica B, vol. 283, 2000, pp.27-31.[42]. Choi, S.U.S., Lee, S., Li, S., Eastman, J.A., “Measuring Thermal Conductivity of Fluids Containing OxideNanoparticles”, Journal of Heat Transfer, vol.121, 1999, pp.280-289.[43]. Eastman, J.A., Choi, S.U.S., Li, S., Thompson, L.J., Lee, S., “Enhanced thermal conductivity throughdevelopment of nanofluids”, Proceedings of Materials Research Society Symposium, Materials ResearchSociety Pittsburgh, PA, USA, Boston, MA, USA, vol.457, 1997, pp. 3-11.[44]. Xue, L., Keblinski, P., Phillpot, S.R., Choi, S.U.S., Eastman, J.A., “Effect of liquid layering at the liquid-solid interface on thermal transport”, International Journal of Heat and Mass transfer, vol.47, 2004, pp.4277-4284.[45]. Xue, Q.Z., “Model for thermal conductivity of Carbon nanotube based composites”, Physica B, vol.368,2005, pp.302-307.[46]. Xue, Q., and Xu, W.M., “A model of thermal conductivity of nanofluids with interfacial shells”, MaterialsChemistry and Physic, vol.90, 2005, pp.298-301.[47]. Ren, Y., Xie, H., Cai, A., “Effective thermal conductivity of Nanofluids containing sphericalNanoparticles”, Journal of Physics D: Apllied Physics, vol. 38, 2005, pp.3958-3961.[48]. Xie, H., Fujii, M., and Zhang, X., “Effects of Interfacial Nanolayer on the effective thermal conductivity ofnanoparticle-fluid mixture”, International Journal of Heat and Mass Transfer, vol. 48, 2005, pp.2926-2932.[49]. Yu, W., Choi, S.U.S., “A effective thermal conductivity model of nanofluids with a cubical arrangement ofspherical particles”, Journal of Nanoscience and Nanotechnology, vol.5, 2007, pp. 580-586.[50]. Garboczi, E.J., Snyder, K.A., Douglas, J.F., “Geometrical percolation threshold of overlapping ellipsoids”,Physical review E, vol.52, 1995, pp.819-828.[51]. Li, Q. and Xuan, Y., “Convective heat transfer and flow characteristics of Cu+ water nanofluids”, Sciencein China, Series E: Technological Sciences, vol. 45, 2002, pp.408-416.[52]. Wang, B., Zhou, L., Peng, X., “Fractal model for predicting the effective thermal conductivity of liquidwith suspension of nanoparticle”, International Journal of heat and mass transfer, vol. 46, 2003, pp.2665-2672.[53]. Gao, L., Zhou, X.F., “Differential effective medium theory for thermal conductivity in nanofluids”,Physics Letters A, vol. 348, 2006, pp.355-360.[54]. Hamilton, R. L., and Crosser, O. K., 1962, “Thermal Conductivity of Heterogeneous Two-ComponentSystems,” Ind. Eng. Chem. Fund., 1(3), pp. 187-191.[55]. Yu, W., and Choi, S. U. S., 2003, “The Role of Interfacial Layers in the Enhanced Thermal Conductivityof Nanofluids: A Renovated Maxwell Model,” J. Nanopart. Res., 5(1), pp. 167-171.[56]. Sitprasert, C., Dechaumphai, P., and Juntasaro, V., 2009, “A Thermal Conductivity Model for NanofluidsIncluding Effect of the Temperature-Dependent Interfacial Layer,” J. Nanopart. Res., 11(6), pp. 1465-1476.[57]. Koo, J., and Kleinstreuer, C., 2004, “A New Thermal Conductivity Model for Nanofluids,” J. Nanopart.Res., 6(6), pp. 577-588.[58]. Oh, D., Jain, A., Eaton, J. K., Goodson, K. E., and Lee, J. S., 2008, “Thermal Conductivity Measurementand Sedimentation Detection of Aluminum Oxide Nanofluids by Using the 3ω Method,” Int. J. Heat Fluid Fl.,29(5), pp. 1456-1461.[59]. Wen, D., and Ding, Y., 2004, “Experimental Investigation into Convective Heat Transfer of Nanofluids atthe Entrance Region under Laminar Flow Conditions,” Int. J. Heat Mass Tran., 47(24), pp. 5181-5188.[60]. Nimtz, G., Marquardt, P., and Gleiter, H., 1990, “Size-Induced Metal-Insulator Transition in Metals andSemiconductors,” J. Cryst. Growth, 86(1-4), pp. 66-71.[61]. Xie, H., Wang, J., Xi, T., Liu, Y., and Ai, F., 2002, “Dependence of the Thermal Conductivity ofNanoparticle-Fluid Mixture on the Base Fluid,” J. Mater. Sci. Lett., 21(19), pp. 1469-1471.[62]. Beck, M., Yuan, Y., Warrier, P., and Teja, A., 2009, “The Effect of Particle Size on the ThermalConductivity of Alumina Nanofluids,” J. Nanopart. Res., 11(5), pp. 1129-1136. 27 Vol. 5, Issue 1, pp. 13-28
- 16. International Journal of Advances in Engineering & Technology, Nov. 2012.©IJAET ISSN: 2231-1963[63]. Chen, H., Witharana, S., Jin, Y., Kim, C., and Ding, Y., 2009, “Predicting Thermal Conductivity of LiquidSuspensions of Nanoparticles (Nanofluids) Based on Rheology,” Particuology, 7(2), pp. 151-157.[64]. Nan, C. W., Shi, Z., and Lin, Y., 2003, “A Simple Model for Thermal Conductivity of Carbon Nanotube-Based Composites,” Chem. Phys. Lett., 375(5-6), pp. 666-669.[65]. Xue Yu, W., and Choi, S., 2004, “The Role of Interfacial Layers in the Enhanced Thermal Conductivity ofNanofluids: A Renovated Hamilton–Crosser Model,” J. Nanopart. Res., 6(4), pp. 355-361.[66]. Xue, Q., 2003, “Model for Effective Thermal Conductivity of Nanofluids,” Phys. Lett. A, 307(5-6), pp.313-317.[67]. Li, Y., Qu, W., and Feng, J., 2008, “Temperature Dependence of Thermal Conductivity of Nanofluids,”Chinese Phys. Lett., 25(9), pp. 3319-3322.[68]. Leong, K., Yang, C., and Murshed, S., 2006, “A Model for the Thermal Conductivity of Nanofluids – TheEffect of Interfacial Layer,” J. Nanopart. Res., 8(2), pp. 245-254.BIOGRAPHICAL NOTESB. Ravi Sankar is currently working as Lecturer in the Department of MechanicalEngineering, R.V.R.&J.C. College of Enigneering, Guntur, Andhra Pradesh,India. Hegraduated in Mechanical Engineering from the same college in 2002. He received his MastersDegree from ANU, India in 2005. He has published 2 research papers in International Journalsand various papers in International and National conferences.D. Nagesawara Rao worked as a Professor in Andhra University, Visakhapatnam, India forpast 30 years and presently he is working as Vice Chancellor, Centurion University ofTechnology & Management, Odisha, India. Under his guidance 18 PhD’s were awarded. Hehas undertaken various projects sponsored by UGC, AICTE and NRB. He worked as acoordinator for Centre for Nanotechnology, Andhra University, Visakhapatnam.Ch. Srinivasa Rao is currently an Associate Professor in the Department of MechanicalEngineering, Andhra University, Visakhapatnam, India. He graduated in MechanicalEngineering from SVH Engineering College, Machilipatnam,, India in 1988. He received hisMasters Degree from MANIT, Bhopal, India in 1991. He received PhD from AndhraUniversity in 2004.He has published over 25 research papers in refereed journals andconference proceedings. 28 Vol. 5, Issue 1, pp. 13-28

No public clipboards found for this slide

×
### Save the most important slides with Clipping

Clipping is a handy way to collect and organize the most important slides from a presentation. You can keep your great finds in clipboards organized around topics.

Be the first to comment